 renormalized. With these two assumptions we can reproduce (i) the positions of the Raman active phonons and their splitting and evolution in the (mechanically detwinned) orthorhombic antiferromagnetic state and (ii) Raman intensities, including the $\tilde{a}-\tilde{b}$ anisotropy as well as the complex resonant evolution with the laser light frequency. This agreement gives an experimental justification to the proposed computational procedure and convincingly substantiates the physical concepts it was derived from, namely the pivotal role of local moments in the lattice dynamics of Fe-based superconductors, and the importance of band renormalizations for $d$-electrons.

![(Color online) FeAs layer of and detwinning clamp. (a) The As-atoms (grey) in the center and at the edges are below and, respectively, above the Fe plane (red). For this reason, the 2Fe unit cell with the axes $a$ and $b$ (green) is determined by the As atoms. In the orthorhombic phase the Fe-Fe distances become inequivalent with the distortion strongly exaggerated here. The magnetic unit cell is twice as large as the 2Fe unit cell and has the axes $\tilde{a}$ and $\tilde{b}$. (b) Schematic sketch and (c) photograph of the detwinning clamp. The sample (4) is glued on the copper plate (1) which is in good thermal contact with the sample holder (3). Upon tightening the screws (5) the force exerted by the copper-beryllium cantilever (2) can be adjusted. (d) Schematic representation of the geometry of our Raman scattering experiment. All incoming light polarizations which are not parallel to $y$ have finite projections on the $c$ axis (red arrow).[]{data-label="fig:orth_phase"}](./Baum_fig1.pdf){width="8.5cm"}

Methods
=======

Samples {#sec:samples}
-------

The crystal was prepared using a self-flux technique. Details of the crystal growth and characterization are described elsewhere.[@Chu:2009] is a parent compound of double-layer iron-based superconductors and orders in a stripe-like spin-density-wave (SDW) below ${\ensuremath{T_\mathrm{SDW}}\xspace}\approx \mathrm{135\,K}$. Superconductivity can be obtained by substituting any of the ions or by pressure.[@Kimber:2009
renormalized. With these two assumptions we can reproduce (i) the positions of the Raman active phonons and their splitting and development in the (mechanically detwinned) orthorhombic antiferromagnetic department of state and (ii) Raman intensities, including the $ \tilde{a}-\tilde{b}$ anisotropy equally well as the complex resonant development with the laser light frequency. This agreement gives an experimental justification to the nominate computational routine and convincingly substantiates the forcible concept it was derived from, namely the pivotal role of local consequence in the lattice dynamics of Fe - based superconductors, and the importance of isthmus renormalizations for $ d$-electrons. 

! [ (Color online) FeAs layer of and detwinning clamp. (a) The As - atoms (grey) in the center and at the edges are downstairs and, respectively, above the Fe plane (red). For this reason, the 2Fe whole cell with the axes $ a$ and $ b$ (green) is determined by the As atoms. In the orthorhombic phase the Fe - Fe distance become inequivalent with the distortion strongly exaggerated here. The magnetic unit cell is doubly as large as the 2Fe unit cell and has the axes $ \tilde{a}$ and $ \tilde{b}$. (b) conventional cartoon and (coulomb) photograph of the detwinning clamp. The sample (4) is glued on the copper plate (1) which is in good thermal contact with the sample holder (3). Upon tightening the prison guard (5) the force exerted by the bull - beryllium cantilever (2) can be adjust. (d) conventional representation of the geometry of our Raman scattering experiment. All incoming light polarizations which are not parallel to $ y$ have finite projections on the $ c$ axis (red arrow).[]{data - label="fig: orth_phase"}](./Baum_fig1.pdf){width="8.5 cm " } 

 method 
 = = = = = = = 

 Samples { # sec: samples } 
 ------- 

 The crystal was prepared using a self - flux proficiency. Details of the crystal growth and characterization are described elsewhere.[@Chu:2009 ] is a parent compound of double - layer iron - establish superconductors and orders in a stripe - like spin - density - wave (SDW) below $ { \ensuremath{T_\mathrm{SDW}}\xspace}\approx \mathrm{135\,K}$. Superconductivity can be obtained by substitute any of the ions or by pressure.[@Kimber:2009
 rejormalized. With these twu assumptions wg xan re'roduce (i) the pusitions of the Raman active pyononw and their splitting xnd evolunion in tye (mtchanically detwiihed) ortmjrhojnic autmferromagnetic xtate and (hi) Raman intenvigizs, including the $\tilde{a}-\tilde{b}$ anisotwopy as wfll as the comklex gefonahn tvolution with the laser light frsquency. This agreememt gives an experimental jkstivication to the prlposed compofatyinal procedufe and connnncingly sugstantiates the physical concepgs it was derivgb frlk, namely thx pivonal role of local momants in the lattice dnnamirs od Fe-based superconducvors, and the importagce of batd renormalizations fir $d$-enectsons.

![(Zilof ohlmne) FeAs payxr of and dstwinning coamp. (a) The As-atoms (brqj) in the centsr and ae the edges are below and, respectively, dbobe the Fe plane (red). For this reason, the 2Fe ujit cell rith the axes $a$ and $b$ (green) is determined by the Ds atkos. Nk gye orthorhombic phase the Fe-Fe distances become jntqupvalent with the bistortion stronblj rvaggerated hete. The maghetic unit cell is twice ws laege as tht 2Fe init cell and has the axes $\rilde{a}$ and $\tplde{v}$. (b) Schematic sketeh and (c) phocograpn of yhe detwinning clamp. Thz sampme (4) is gluef on the dupper plate (1) whizh ps it good thermal contact witr the sam'le hplder (3). Jpon tightqning the dcrews (5) the force exertef by jhe co[per-berylllum cantilever (2) can be adjusted. (d) Schematic rgprasettation jf thc geometry of otr Raman scattgring expzrimeng. All incojing lijht polarizaeions which asg not parallen to $y$ hwve dinire projdztions on the $v$ axis (reb arriw).[]{data-label="fig:orth_ihase"}](./Czum_fig1.pdf){width="8.5cn"}

Meuhids
=======

Samples {#sec:xamolef}
-------

Tje cwfstal was prapardd jxing x self-flux becfniqie. Details of the crfstam growth and charavtcrization are dessribed elsewhrre.[@Chu:2009] is a parent compmunv of dpubje-layer iron-based superconductkrs and ogdevs in a stripq-likc spyn-density-wcve (SDW) below ${\ensuremath{T_\mathrm{SDW}}\xspace}\epprox \mathrm{135\,K}$. Superconeuctivity can be objaiked by substmtutind any of dhe ions or by pressyre.[@Kimber:2009
renormalized. With these two assumptions we can the of the active phonons and the detwinned) orthorhombic antiferromagnetic and (ii) Raman including the $\tilde{a}-\tilde{b}$ anisotropy as well the complex resonant evolution with the laser light frequency. This agreement gives an justification to the proposed computational procedure and convincingly substantiates the physical concepts it derived namely pivotal of local moments in the lattice dynamics of Fe-based superconductors, and the importance of band renormalizations $d$-electrons. ![(Color online) FeAs layer of and detwinning (a) The As-atoms (grey) the center and at the are and, respectively, the plane For this reason, 2Fe unit cell with the axes $a$ and $b$ (green) is determined by the As atoms. In orthorhombic phase distances become with distortion exaggerated here. The cell is twice as large as cell and has the axes $\tilde{a}$ and $\tilde{b}$. Schematic sketch (c) photograph of the detwinning clamp. sample (4) is glued on the copper plate which is in good thermal contact with the sample holder (3). Upon tightening the screws force exerted by the cantilever (2) can adjusted. Schematic of geometry of Raman scattering experiment. All incoming light polarizations which are not parallel $y$ have finite projections on the $c$ axis (red arrow).[]{data-label="fig:orth_phase"}](./Baum_fig1.pdf){width="8.5cm"} Samples ------- The crystal prepared using a self-flux Details the crystal growth and described is of iron-based and orders in a spin-density-wave (SDW) below ${\ensuremath{T_\mathrm{SDW}}\xspace}\approx \mathrm{135\,K}$. can be obtained by or by pressure.[@Kimber:2009
 renormalized. With these two aSsumptions We can RepRodUcE (i) thE posItions of the RamAN actIve phonons and their spliTting AnD EvolUTiOn in tHe (mechaNIcALLy dEtWiNneD) oRThOrhomBic AntiferRomagnetic StaTe And (ii) Raman inTEnSities, inclUdiNg the $\tilde{a}-\tIldE{b}$ anisOtRopY As welL as The coMplex rESonant Evolution WiTH the laSEr light FREqUencY. This agreement givES aN Experimental juStificAtIOn TO The ProPosed compuTaTionaL ProceduRE aND COnvINcingly substaNtiates the pHYsiCal conCePts IT was deRived FrOM, naMely the pivoTal rOle of locaL momenTS in the lATtice dyNamics Of FE-baSed sUPeRcOndUcTOrs, ANd The IMpoRtance of BaNd RenorMaliZATIOns fOr $d$-ElecTrons.

![(color online) Feas lAyer OF anD detwInninG claMp. (A) The AS-atoms (Grey) iN tHe center and at thE edgEs are beloW anD, rEspEcTivelY, Above tHe FE plAne (red). FOr this rEAsoN, tHE 2fE uNit cell with the axes $A$ aND $B$ (gReen) is deTerminED bY tHE As atoms. in The OrthORHombiC phaSE tHe Fe-Fe diStanceS BeCoMe inequIvAlent wItH thE diStortIOn stRongly ExaggeraTed heRE. The magnetic unIT cell is twice aS LaRGE aS The 2FE unIt cell and haS the AXes $\tIlde{A}$ AnD $\tiLDe{b}$. (b) SChemaTiC SkETch and (c) photograph of ThE detwiNning Clamp. The samplE (4) is glued on THE Copper plAte (1) wHIcH Is in good thermaL contAct with the SAmple holDer (3). UpOn tighteNing the scREWs (5) the forCe eXerTed By tHE CoPper-beryllium CANtilEvEr (2) can be AdjUsted. (d) SCheMatIc rEprEsEntation oF the geomEtRy Of OuR RaMan scATtering eXpEriMeNt. ALl incOMing liGht poLariZaTiONs wHich are NOt PARallEl To $Y$ havE fiNiTe proJectIOns On the $c$ aXis (red arrOw).[]{dATa-laBeL="fIg:orth_pHase"}](./Baum_fig1.pdF){wIdth="8.5cm"}

MethOdS
=======

SaMples {#sEC:Samples}
-------

THe crystal was prepared usiNG a self-fLux TechnIque. details of The CrystaL grOWth and CharacTerizAtIon ARE descRIBeD elSeWhere.[@Chu:2009] is A PAreNt comPoUnd oF double-Layer iron-based supeRConDuctors and ordErs In a sTRIpE-liKE sPIn-dEnSIty-WAVe (SDW) below ${\ensurEmath{T_\mathRm{sdW}}\Xspace}\apprOX \maThRm{135\,K}$. SupeRconducTivitY Can be obTained by sUbstitutiNg Any oF THe iOns or by preSsure.[@KimBer:2009
 renormalized. With thesetwo assump tions  we  ca nrepr oduc e (i) the posi t ions  of the Raman active p honon sa nd t h ei r spl ittinga nd e vol ut io n i nt he  (mec han icallydetwinned)  or th orhombic ant i fe rromagneti c s tate and (ii ) R aman i nt ens i ties,  in cludi ng the $\tild e{a}-\til de { b}$ an i sotropy a swell  as the complex r e so n ant evolutionwith t he la s e r l igh t frequenc y.  This agreeme n tg i v esa n experimenta l justifica t ion  to th epro p osed c omput at i ona l procedure  and  convinci ngly s u bstanti a tes the  physi cal  co ncep t sit  wa sd eri v ed  fr o m,namely t he  p ivota l ro l e o f lo cal  mom entsin the lattic e d ynam i csof Fe -base d su pe rcond uctors , and  t he importance o f ba nd renorm ali za tio ns  for$ d$-ele ctr ons .

![(C olor on l ine )F e A slayer of and detwi nn i n gclamp. ( a) The As -a t oms (gre y)  in  the c enter  and at  the edg es are be lo w and,re specti ve ly,  ab ove t h e Fe  plane  (red).For t h is reason, the 2Fe unit cell wi t h  t h e ax es$a$ and $b$  (gr e en)is d e te rmi n ed by  theAs at o ms. In the orthorho mb ic pha se th e Fe-Fe dista nces becom e i nequival entw it h  the distortio n str ongly exag g erated h ere.The magn etic unit c ell is t wic e a s l arg e as  the 2Fe unit c ellan d has t heaxes $\ til de{ a}$  an d$\tilde{b }$. (b)Sc he ma ti c s ketch and (c)ph oto gr aph  of t h e detw innin g cl am p. The  sample (4 ) is g lu ed  onthe  c opper  pla t e ( 1) whic h is in g ood ther ma lcontact  with the sam pl e holder ( 3) . U pon ti g h tening t he screws (5) the force exerted  by  thecopp er-beryll ium  canti lev e r (2)can be  adju st ed. ( d) Sc h e ma tic  r epresentat i o n o f the  g eome try ofour Raman scatteri n g e xperiment. Al l i ncom i n glig h tp ola ri z ati o n s which are not  parallelto $y $ have fin i tepr ojectio ns on t he $c $  axis ( red arrow ).[]{data -l abel = " fig :orth_phas e"}](./B aum_fig1. p df){w i dt h="8. 5cm "}

Me th ods 
==== ===

S a mpl es {# sec:sa mp les}
- ----- -
The cry stal was prepared using  a sel f-flu x t echnique.  De t ail s of thecrys tal growth  an d c harac ter i zatio n ar e  d esc r ibedelse w here.[@Ch u :2 009 ] is  a parent c o m p oun d ofdou b le-lay er i ron-based superco n ductors and or ders i n a  st r ipe- li ke spin-densit y-w av e (SDW) be lo w ${\ensure math{T_\ ma t hrm{S DW}}\x space} \approx \ ma t hrm{13 5\,K }$.  Supercon duc ti v ity can  b eo btaine d by  s ubstit utinga ny o f the ions or by p ressu r e .[@Ki m ber :2009 
 renormalized._With these_two assumptions we can_reproduce (i)_the_positions of_the_Raman active phonons_and their splitting_and evolution in the_(mechanically detwinned) orthorhombic_antiferromagnetic_state and (ii) Raman intensities, including the $\tilde{a}-\tilde{b}$ anisotropy as well as the complex_resonant_evolution with_the_laser_light frequency. This agreement gives_an experimental justification to the_proposed computational_procedure and convincingly substantiates the physical concepts it_was_derived from, namely_the pivotal role of local moments in the lattice_dynamics of Fe-based superconductors, and the_importance of band_renormalizations_for_$d$-electrons.

![(Color online) FeAs layer_of and detwinning clamp. (a) The_As-atoms (grey) in the center and_at the edges are below and, respectively,_above the Fe plane (red). For_this reason, the 2Fe unit_cell with_the axes $a$ and $b$_(green) is determined_by the_As atoms. In_the orthorhombic phase the Fe-Fe distances_become inequivalent with_the distortion strongly exaggerated here. The_magnetic_unit cell is_twice_as_large as_the 2Fe unit_cell_and has_the_axes $\tilde{a}$ and $\tilde{b}$. (b) Schematic_sketch_and (c) photograph of the detwinning clamp._The sample (4) is_glued_on the copper plate_(1) which is in good_thermal contact with the sample holder_(3). Upon_tightening the_screws (5) the force exerted by the copper-beryllium cantilever (2) can_be adjusted. (d) Schematic representation of_the geometry of our_Raman scattering_experiment._All incoming light_polarizations_which are_not parallel to $y$ have finite projections_on the_$c$ axis (red arrow).[]{data-label="fig:orth_phase"}](./Baum_fig1.pdf){width="8.5cm"}

Methods
=======

Samples {#sec:samples}
-------

The crystal_was prepared using a_self-flux_technique. Details of the crystal growth_and characterization are described elsewhere.[@Chu:2009] is_a parent compound of double-layer_iron-based_superconductors_and orders in a stripe-like_spin-density-wave (SDW) below ${\ensuremath{T_\mathrm{SDW}}\xspace}\approx \mathrm{135\,K}$. Superconductivity_can be obtained_by substituting any of the ions or_by_pressure.[@Kimber:2009